Reversible Capture and Release of Cl and Br with a web.mit.edu/dincalab/papers/ Reversible Capture...
Embed Size (px)
Transcript of Reversible Capture and Release of Cl and Br with a web.mit.edu/dincalab/papers/ Reversible Capture...
Reversible Capture and Release of Cl2 and Br2 with a Redox-Active Metal−Organic Framework Yuri Tulchinsky,† Christopher H. Hendon,† Kirill A. Lomachenko,§,∥ Elisa Borfecchia,⊥ Brent C. Melot,‡
Matthew R. Hudson,# Jacob D. Tarver,#,∇ Maciej D. Korzynśki,† Amanda W. Stubbs,† Jacob J. Kagan,○
Carlo Lamberti,⊥,∥ Craig M. Brown,# and Mircea Dinca*̆,†
†Department of Chemistry, Massachusetts Institute of Technology, 77 Massachusetts Avenue, Cambridge, Massachusetts 02139, United States ‡Department of Chemistry, University of Southern California, 3620 McClintock Avenue, Los Angeles, California 90089-1062, United States §European Synchrotron Radiation Facility, 71 Avenue des Martyrs, CS 40220, 38043 Grenoble Cedex 9, France ∥IRC “Smart Materials”, Southern Federal University, Zorge Street 5, 344090 Rostov-on-Don, Russia ⊥Department of Chemistry, NIS, CrisDi, and INSTM Centre of Reference, University of Turin, Via Quarello 15, I-10135 Torino, Italy #Center for Neutron Research, National Institute of Standards and Technology, Gaithersburg, Maryland 20899, United States ∇National Renewable Energy Laboratory, 15013 Denver West Parkway, Golden, Colorado 80401, United States ○Department of Mathematics, Weizmann Institute of Science, 234 Herzl Street, Rehovot 7610001, Israel
*S Supporting Information
ABSTRACT: Extreme toxicity, corrosiveness, and volatility pose serious challenges for the safe storage and transportation of elemental chlorine and bromine, which play critical roles in the chemical industry. Solid materials capable of forming stable nonvolatile compounds upon reaction with elemental halogens may partially mitigate these challenges by allowing safe halogen release on demand. Here we demonstrate that elemental halogens quantitatively oxidize coordinatively unsaturated Co(II) ions in a robust azolate metal−organic framework (MOF) to produce stable and safe-to- handle Co(III) materials featuring terminal Co(III)−halogen bonds. Thermal treatment of the oxidized MOF causes homolytic cleavage of the Co(III)−halogen bonds, reduction to Co(II), and concomitant release of elemental halogens. The reversible chemical storage and thermal release of elemental halogens occur with no significant losses of structural integrity, as the parent cobaltous MOF retains its crystallinity and porosity even after three oxidation/reduction cycles. These results highlight a material operating via redox mechanism that may find utility in the storage and capture of other noxious and corrosive gases.
■ INTRODUCTION Elemental halogens play key roles in a range of industrial processes. With an estimated annual production of 56 million tons, Cl2 is widely used in water sanitation and is an essential ingredient in the production of plastics, such as poly(vinyl chloride) and polyurethanes, as well as solvents and pesticides.1
Although used on a comparatively smaller scale, Br2 is a key element in flame retardants, agricultural products, and pharmaceuticals.2 The irreplaceable role of the elemental halogens in industry is contrasted with their extreme toxicity, corrosiveness, and volatility, which pose serious challenges for their safe handling, storage, and transportation. Despite decades of experience in mitigating these challenges, tragic accidents still occur worldwide as a result of leaks or explosions, making the development of new materials that can enable the open-air, safe-handling, and on-demand delivery of halogens highly
desirable. Metal−organic frameworks (MOFs), with their demonstrated utility in storing both inert and reactive gases, seem like logical choices for this challenge. However, despite thousands of reports on gas sorption and storage in MOFs, many including oxidizing or corrosive gases such as O2,
SO2, 6,7 and NH3,
7−10 to our knowledge none address the reversible storage of Br2 or Cl2. The closest example is the irreversible bromination of an unsaturated organic ligand within a MOF and subsequent release of HBr upon treatment with base.11 The lack of reports on reversible storage of the gaseous halogens (i.e., excluding I2) in MOFs is staggering given the interest in the field, but it highlights the difficulty in isolating
Received: March 7, 2017 Published: March 28, 2017
© 2017 American Chemical Society 5992 DOI: 10.1021/jacs.7b02161 J. Am. Chem. Soc. 2017, 139, 5992−5997
materials that can reversibly bind halogens and release them over at least several cycles. Although physisorption is the most widely employed
mechanism for gas storage in porous materials, it is less effective with the lighter halogens because gas retention under ambient conditions is relatively poor and thus still requires the use of specialized storage and handling equipment. One historical shortcoming of MOFs for this application is their chemical instability toward Cl2 and Br2. With reports of reversible redox cycling of MOFs,12,13 we became intrigued by a chemical storage mechanism whereby Cl2 and Br2 could be stored by reduction to Cl− and Br− and subsequently released by oxidation back to their elemental X2 form. Here we report such a mechanism, where elemental Br2 and Cl2 reversibly oxidize Co(II) centers in Co2Cl2BTDD (1) (BTDD = bis(1H- 1,2,3-triazolo[4,5-b],[4,5-i])dibenzo[1,4]dioxin) to form termi- nal cobalt(III) halides in Co2Cl2X2BTDD (X = Cl (2), Br (3)).
To our knowledge, these are the first examples of all-Co(III) MOFs. We show that the Co(III) materials can be reduced back to Co(II) thermally, with concomitant liberation of X2. These results represent the first example of reversible halogen uptake and release with a MOF and portend applications for halogen capture in the context of toxic gas removal and halogen storage in the context of safe handling of halogens.
■ RESULTS AND DISCUSSION Robust Reactivity with Elemental Halogens and
Formation of All-Co(III) MOFs. Reaction of H2BTDD with CoCl2·6H2O results in the formation of solvated Co2Cl2BTDD (1), as previously described.10 Rietveld analysis of neutron powder diffraction (NPD) data obtained from a sample of activated 1 at 10 K revealed a three-dimensional structure exhibiting one-dimensional channels arranged in a honeycomb fashion, similar to that reported for the Mn analogue
Figure 1. Structural and microscopy data. (A) A portion of the structure of the parent Co(II) MOF Co2Cl2BTDD (1) projected along the c axis. (B−D) SBU structures and local coordination environments of the Co centers in 1, 2, and 3, respectively, as determined by NPD. (E) PXRD data for 1, 2, and 3 showing retention of crystallinity and the lattice contraction in moving from 1 to 2 and 3, as evidenced by the upshift in the 2θ values for the (2-10) and (300) reflections. (F−H) Scanning electron micrographs of microcrystalline samples of 1, 2, and 3, respectively.
Figure 2. Co K-edge XAS characterization of 1 and 2. (A) (top) Theoretical XANES spectra for 1 and 2 calculated from the NPD structures. (bottom) Experimental XANES spectra at room temperature (RT) for 1, 2, 2 after heating, and intermediate states collected in situ in the 200−290 °C range during the thermal treatment of 2; the inset shows a magnification of the pre-edge peak at ca. 7709 eV. (B) Magnitudes and (C) imaginary parts of the phase-uncorrected Fourier transformed k2-weighted EXAFS spectra, FT(R). (D) Linear combination analysis of the whole series of in situ XANES spectra using the spectra of 1 and 2 at RT as references: relative fraction (open symbols) and fit quality factor (solid symbols).
Journal of the American Chemical Society Article
DOI: 10.1021/jacs.7b02161 J. Am. Chem. Soc. 2017, 139, 5992−5997
Mn2Cl2BTDD. 10 The secondary building units (SBUs) of 1
consist of infinite −(Co−Cl)n− chains coiled into threefold spirals and interconnected by the bis(triazolate) linkers (Figure 1A). Reaction of olive-green rodlike microcrystals of 1 with gaseous Cl2 or PhICl2 in dichloromethane results in rapid oxidation and quantitative formation of dark-brown micro- crystals of Co2Cl4BTDD (2) (Figure 1B). A powder X-ray diffraction (PXRD) pattern of 2 revealed small but noticeable shifts in all of the reflection peaks toward higher scattering angles (2θ). These were most evident in the peaks corresponding to the (21 ̅0) and (300) reflections (Figures 1C and S1), which shift from 4.5° and 7.8° in 1 to 4.6° and 8.0° in 2, respectively. NPD analysis of 2 revealed decreases of 0.13 and 0.14 Å in the average Co−N and Co−Cl bond lengths, respectively, relative to those in 1, as expected upon oxidation of Co(II) sites in 1 to Co(III) in 2. The stoichiometry of the oxidation of 1 to 2 in the presence
of Cl2 or PhICl2 was ascertained by microelemental analysis (see the Supporting Information), X-ray absorption spectros- copy (XAS), and magnetometry. X-ray absorption near-edge spectroscopy (XANES) at the Co K-edges of 1 and 2 at room temperature revealed that the absorption edge of 2 is shifted by approximately 2 eV to higher energy relative to that of 1 (Figure 2A).14,15 Although this shift cannot be used to quantify the degree of oxidation in 1, it does indicate a higher average effective nuclear charge on the metal. This confirms that oxidation indeed takes place at the Co centers and not at the ligand, as had been previously observed, for instance, with the topologically related Mn2(2,5-dihydroxyterephthalate) (Mn- MOF-74) under similar oxidation conditions.16 Magnetic measurements were particularly useful in determining whether the oxidation of Co(II